**HAL Id: hal-01006930**

**https://hal.archives-ouvertes.fr/hal-01006930**

### Submitted on 21 Nov 2016

**HAL is a multi-disciplinary open access**

### archive for the deposit and dissemination of

### sci-entific research documents, whether they are

### pub-lished or not. The documents may come from

### teaching and research institutions in France or

### abroad, or from public or private research centers.

**L’archive ouverte pluridisciplinaire HAL, est**

### destinée au dépôt et à la diffusion de documents

### scientifiques de niveau recherche, publiés ou non,

### émanant des établissements d’enseignement et de

### recherche français ou étrangers, des laboratoires

### publics ou privés.

### Distributed under a Creative Commons Attribution| 4.0 International License

**Homogenization of corrugated core sandwiches panels**

### Natacha Buannic, Patrice Cartraud, Tanguy Quesnel

**To cite this version:**

### Natacha Buannic, Patrice Cartraud, Tanguy Quesnel. Homogenization of corrugated core sandwiches

### panels. Composite Structures, Elsevier, 2003, 59 (3), pp.298-311. �10.1016/S0263-8223(02)00246-5�.

### �hal-01006930�

## Homogenization

## of corrugated core sandwich panels

### Natacha

### Buannic

a### ,

### Patrice Cartraud

b### ,

### Tanguy Quesnel

a_{Principia Marine, 1 Rue de la Noee, B.P. 72108, 44321 Nantes Cedex 3, France}
b_{Laboratoire M}

eecanique et Mateeriaux, Ecole Centrale de Nantes, 1, Rue de la Noe, B.P. 92101, 44321 Nantes Cedex 3, France

The present work is devoted to the computation of the eﬀective properties of corrugated core sandwich panels. Due to their periodic structure, the homogenization theory is used, based on the asymptotic expansion method. At the leading order, an equivalent Kirchhoﬀ Love homogeneous plate is derived, with an overall behavior obtained from basic cell problems posed on the three dimensional period of the panel. The ﬁnite element computation of these eﬀective properties is presented in this paper. The accuracy of the homogenization method is proved, since the real panel and equivalent plate responses are very close for membrane and pure bending loadings. However, a discrepancy appears for simple bending loading, underlining that transverse shear eﬀects cannot be neglected. Therefore, a speciﬁc study is developed in order to derive the transverse shear stiﬀness, thus enabling to de termine an equivalent Reissner Mindlin homogeneous plate.

Keywords: Homogenization; Eﬀective stiﬀness; Corrugated core; Sandwich panel; Finite element method

1. Introduction

Sandwich structural panels are widely used in many industrial areas, and the purpose of the present paper is to investigate their applications in shipbuilding, as an alternative to stiﬀened panels.

To this aim, a comparative study of diﬀerent panels will be made with respect to a reference stiﬀened panel similar to those traditionally used in shipbuilding. The analysis will be limited to their ratios stiﬀness over mass.

The sandwich panels considered here are corrugated core sandwich panels, the core and the facings being made of steel. Four diﬀerent core shapes were selected for this study, owing to their easy manufacturing by laser welding. The unidirectional corrugated core is: (a) straight, (b) of hat type, (c) triangular or (d) curvilinear. The stiﬀened panel (e) used as a reference in the study is also presented in Fig. 1.

Several approaches to the modeling of these struc-tural elements are discussed in the literature, see e.g. the review article [1].

For instance, a three-dimensional (3D) ﬁnite element model can be used, where the actual geometry of the core is represented. However, such a model is bound to have a high computational cost, and is inadequate when one is interested in the overall response of the structure. At the scale of a ship, these panels present indeed an overall plate-like behavior, and the problem is then to deﬁne the eﬀective plate stiﬀnesses.

Several authors proposed to use an equivalent con-tinuum instead of the core, and then combine it with a 3D model [2] or a bidimensional plate model [3] (in both references, a honeycomb core is considered. For a va-riety of cellular core geometries, see the recent review article [4]). In the plate model, the sandwich is then modeled as several layers, and some approximations are made in the direction of the thickness. This type of ap-proach was used among other things for the corrugated cores that are of interest here. Then, from a strength-of-materials type of theory, analytical expressions for the characteristics of the equivalent continuum are given in [5,6]. Diﬀerent geometries of corrugation are studied in the latter reference.

Another approach consists in using the homogeni-zation theory, taking beneﬁt from the periodicity ex-hibited by the structure in its plane. Consequently, the basic cell is made of the core and the facings, i.e. the core is not considered independently. At this stage, it is

noteworthy that the panels studied here are thin 3D structures with periodic microstructure in direction 1, and invariant in direction 2 of plane (x1, x2). These

panels are therefore a special case of panels with peri-odic components in both directions of the plane. Such structures are characterized by the existence of two small parameters noted e and e: e is the ratio between panel thickness t and a characteristic dimension L of the panel in its plane, and e is the ratio between period length X1

or X2 and L (see Fig. 2).

The purpose of homogenization is then to substitute the thin initial heterogeneous structure with an equiva-lent homogeneous plate. This leads to making the two small parameters of the problem tend to zero. This ap-proach was studied theoretically by Caillerie [7], where it was shown that depending on the order in which the two small parameters tend to zero, namely, one after the other or both simultaneously, varied results can be ob-tained for the eﬀective stiﬀnesses. Therefore, several homogenization methods are available, with their own domain of validity. Our objective here is not to discuss these diﬀerent methods, but its interesting to note that replacing the core by an equivalent medium amounts to

make e! 0 ﬁrst, and then e ! 0 using an appropriate sandwich plate theory. The interested reader is referred to the book of Lewinski and Telega [8], where the methods are widely presented, and to [9,10]. In [8], the diﬀerent methods are applied to the bending of a sym-metric stiﬀened panel, and in [9 11] to the membrane and bending behaviors of plates with honeycomb core and of corrugated plates with straight unidirectional stiﬀeners.

In practice, the choice of a homogenization method is dictated by the value of ratio e=e. The panels studied here have values of e and e that are on the same order of magnitude. From a classical study of a heterogeneous plate made of a large number of basic cells, one can identify the equivalent characteristics of the plate. Then, by comparing these characteristics and those given by diﬀerent homogenization methods, it appears that the most accurate results are obtained when both small parameters simultaneously become vanishingly small [10]. This is in the same line as the conclusion drawn in [8]. The latter method will therefore be used here.

This method was initially presented in [7] and is ex-posed in detail in [8]. A similar approach was proex-posed in [12] to study the bending of symmetric plates with a variable thickness. In concrete terms, the homogeniza-tion method involves basic cell problems posed on the 3D period of the panel, i.e. including both the core and the facings. Therefore, as noted in [11], this method is more appropriate than the homogenization of the core into an equivalent medium separately (see [4] for cellular sandwich cores), even if the latter may incorporate core face sheet constraints [13].

Solving the basic cell problems provides the plate eﬀective properties according to a Kirchhoﬀ Love model. In the literature, approximated analytical solu-tions to the cell problems were presented in [8] for uni-directional periodic plates, and in [14 16] for various applications (stiﬀened plates, sandwich plates with honeycomb core and ﬁber reinforced plates).

The cell problems can also be solved numerically using a ﬁnite element model of the basic cell. One can ﬁnd such results in [12] for the bending of symmetric stiﬀened plates, in [17] for unidirectional periodic plates and in [9 11] for plates with straight unidirectional stiﬀeners or honeycomb core. This method of resolution presents the advantage that it can be applied to any type of period and this approach was adopted here.

In the present work, the homogenization theory, based on the asymptotic expansion method, will brieﬂy be described in Section 2. The basic cell problems and their numerical implementation will be presented shortly after. Then, in Section 3, the homogenization method will be applied to the diﬀerent panels shown in Fig. 1. By comparing the response of the equivalent homogeneous plates with that given by detailed ﬁnite element models of sandwich panels, the accuracy of the method will be Fig. 2. Type of panel studied.

(a) Straight
(b) Hat type
(c) Triangular
(d) Curvilinear _{1}
2
3

(e) Reference stiffened panel

Fig. 1. Core shapes of sandwich panels of interest and traditional stiﬀened panel.

demonstrated in Section 4 for in-plane and pure bending types of loading. In Section 5, the eﬀective properties of a ﬁber-reinforced plastic (FRP) honeycomb sandwich panel are computed and compared to those given in [18], in order to show the applicability of the homogenization method presented in this paper to such structures.

The main limitation of the homogenization method used here is that, at the leading order, it leads to an equivalent Kirchhoﬀ Love homogeneous plate. For the structures studied in the present paper, it is likely that such a model will not be totally satisfactory. This problem will be dealt with in Section 6, where a simple method will be proposed to obtain the panel eﬀective transverse shear stiﬀness, and ﬁnally get the properties of an equivalent Reissner Mindlin homo-geneous plate.

The summation convention on repeated indices will
be used throughout the paper. The Latin indices range
from 1 to 3, whereas the Greek indices range from 1 to 2.
In addition, dots and semi-colons will respectively note
the scalar and double products of tensors, e.g.:
ðr nÞ_{i}¼ rijnjandða : eÞij ¼ aijklekl.

2. The homogenization method

2.1. Main results

Following [7,8,10], the main steps of the homogeni-zation method are exposed in this section.

The starting point is the formulation of the 3D problem of a thin structure with in-plane periodic components (the general case of a periodic structure in both directions of its plane is studied here). As men-tioned in introduction, this problem involves two small parameters: e, which corresponds to the slenderness of the structure, and e, associated to the rapid periodic variation of the material and geometrical properties in the in-plane directions. These two small parameters are of the same order of magnitude and are assumed to be equal. Thus, one can use the asymptotic expan-sion method with one small parameter for periodic plates.

Firstly, two scales are introduced: a microscopic one, which is the scale of the heterogeneities and of the thickness, and a macroscopic scale on which the size of the basic cell is very small. The corresponding variables are respectively: yi¼ xi=e and ðz1; z2Þ ¼ ðx1; x2Þ, where

ðxÞ ¼ ðx1; x2; x3Þ is the initial 3D variable. The operators

of the 3D elasticity problem are then expressed as functions of these new variables. Next, the solution of this problem is searched under the form:

uðxÞ ¼ u0_{ðz}

1; z2Þ þ eu1ðz1; z2; y1; y2; y3Þ

þ e2_{u}2_{ðz}

1; z2; y1; y2; y3Þ þ ð1Þ

where functions ui_{ðz}

1; z2; y1; y2; y3Þ are Y1and Y2-periodic

in variable y, Ya¼ Xa=ebeing a length of the period or

basic cell Y at the microscopic scale, see Fig. 2.
It will be considered that the ﬁrst term u0_{ðz}

1; z2Þ of the

expansion in Eq. (1) has only a component in direction 3, which amounts to assuming that the plate bending is prominent, the terms relative to the in-plane displace-ment being of the 1th order in e, that is u0

a¼ 0.

It then turns out that the 3D elasticity problem splits in a sequence of 2D microscopic problems, posed on the basic cell, and 2D macroscopic problems providing the overall plate response.

The main results of the method are now recalled, for more details, see [7,8,10]:

• The solution of the leading order ()1th order)
micro-scopic problem is (the solution is unique up to an
ad-ditive constant ^uu1_{, which corresponds to a rigid body}

translation): u1 i ¼ ^yy3 ou0 3 oza diaþ ^uu1iðz1; z2Þ ð2Þ

where dia is the Kronecker symbol, and where ^yy3¼

y3 yy3 with yy3¼ ð1=jY jÞ

R

Y y3dy1dy2dy3, and jY j

represents the volume of the solid part Y _{of Y. Then,}

^

yy_{3}is the distance in direction 3 from the mid-plane of
the panel, such that y3¼ yy3 or ^yy3¼ 0. In the

follow-ing, the overall plate behavior will be formulated with respect to the mid-plane.

• The leading order macroscopic problem generalizes the Kirchhoﬀ Love theory, the transverse and in-plane displacements being u3

0and ^uu1a. The

correspond-ing homogenized (or eﬀective) constitutive relations are obtained from the solution of the 0th order mi-croscopic problem, which will be exposed in Section 2.2.

2.2. The basic cell problems

Let us introduce membrane macrodeformations E and curvature macrodeformations K deﬁned as:

Eab¼ ezabð^uu
1_{Þ}
Kab¼
o2_{u}3
0
ozaozb
8
<
: ð3Þ

where ez denotes the strain operator corresponding to

the macroscopic variable z.

The 0th order microscopic problems are posed on the basic cell (see Fig. 2). The upper and lower facings are respectively notedoYþandoY, whileoY1stands for the

internal surfaces, which are not loaded. Denoting a the elastic moduli tensor, divy and ey the divergence and

strain operators with respect to the microscopic variable
y, the basic cell problems consist in ﬁnding the ﬁelds uper_{,}

divyr1¼ 0
r1_{¼ aðyÞ : e}
eab ¼ Eabþ ^yy3Kabþ eyabðu
per_{Þ}
ei3¼ eyi3ðu
per_{Þ}
r1_{ n ¼ 0} _{on} _{oY}
[ oY1
uper_{y}

1y2 per and r1 n anti-per

8 > > > > > > < > > > > > > : ð4Þ

where ÔperÕ means Y1and Y2-periodic in variable y, and

anti-per means that r1_{ n are opposite on opposite sides}

ofoY .

The data of problem (4) are the macrodeformations E and K, and due to linearity, its solution is, up to a constant for the displacement:

u2_{i} ¼ vEab
i ðyÞEabþ v
Kab
i ðyÞKab
r1
ij¼ FijabEabþ GijabKab
Fijab¼ aijkl
ovEab_{k}
oyl þ aijab
Gijab¼ aijkl
ovKab_{k}
oyl þ ^yy3aijab
8
>
>
>
>
>
<
>
>
>
>
>
:
ð5Þ

The overall plate behavior is deﬁned from the
mac-roscopic in-plane stress resultants and stress couples
associated with r1_{. The latter are obtained through }

in-tegration over the thickness and calculated using the
following averaging method in period mid-plane ^yy_{3}¼ 0:

N1 ab ¼ hr 1 abi; M 1 ab¼ h^yy3r1abi hi ¼ 1 jY j R Y dy1dy2dy3 withjY j ¼ Y1Y2 ( ð6Þ The homogenized constitutive equation can then be put in the form:

fN1_{g}
fM1_{g}
¼ ½A ½B
½Bt ½D
fEg
fKg
ð7Þ
with the matrices ½A, ½B, ½D easily obtained from the
tensors F and G introduced in Eq. (5), and the
expres-sions given in Eq. (6).

Obtaining functions vEab _{and v}Kab _{requires to solve 6}

cell problems similar to problem (4), where one succes-sively considers that the only non-zero data is a com-ponent of the membrane macrodeformation E or curvature K.

2.3. Numerical solving of homogenization problems The basic cell problems (4) have the same character-istics as those dealt with for the homogenization of the elastic behavior of periodic composite materials (mac-roscopic deformation, periodicity conditions), and for which diﬀerent ﬁnite element solution approaches are available in the literature [19 23].

One can mainly distinguish 2 solution techniques for
the cell problems, both of them using the ﬁnite element
method. The ﬁrst technique consists in taking
mac-rodeformations as problem input data and in working
with stress ﬁeld s1_{¼ aðyÞ : e}

yðuperÞ. The

macrodeforma-tions amount to body forces and surface loads on the

edges, and the calculation of the global force vector is therefore rather tedious.

As a result, we chose a second technique, where one
considers a stress ﬁeld r1_{, and whose starting point is the}

following variational formulation of problem (4):
Find uper _{y}

1y2 per and E; K such that8~uuy1y2 per

and eEE; eKK R

Y ðeEEþ y3KKeþ eyð~uuperÞÞ : a : ðE þ y3Kþ eyðuperÞÞ

dy¼ jY jðeEE : N1_{þ e}_{K}_{K : M}1_{Þ}
8
>
>
>
<
>
>
>
:
ð8Þ
This technique was initially described in [20] for
com-posite materials, and was used in [9,10] for plate
prob-lems. The discretized ﬁeld at the ﬁnite element level is
uper_{, but macroscopic deformations E and K are }

con-sidered as additional degrees of freedom. These macro-scopic degrees of freedom are associated with a virtual node connected to all the elements of the mesh. The matrix relation between the deformations and the de-grees of freedom of the elements is then modiﬁed to satisfy Eq. (4)3 and (4)4 as shown below (letfupere g

de-note the degrees of freedom associated with uper _{for the}

element considered):
e11
e22
e33
2e12
2e23
2e13
8
>
>
>
>
>
>
<
>
>
>
>
>
>
:
9
>
>
>
>
>
>
=
>
>
>
>
>
>
;
¼ ½B
1 0 0 yy^_{3} 0 0
0 1 0 0 yy^_{3} 0
0 0 0 0 0 0
0 0 1 0 0 yy^_{3}
0 0 0 0 0 0
0 0 0 0 0 0
2
6
6
6
6
6
6
4
3
7
7
7
7
7
7
5
2
6
6
6
6
6
6
4
3
7
7
7
7
7
7
5
fuper
e g
fEg
fKg
8
<
:
9
=
;
ð9Þ
where ½B is the element usual matrix, and fEgt¼ fE11;

E22;2E12g, fKgt¼ fK11; K22;2K12g.

At this stage, let us recall that the origin of ^yy_{3}
cor-responds to the reference plane with respect to which the
homogenized characteristics are obtained.

On the other hand, the periodicity of uper_{is taken into}

account by eliminating the redundant degrees of free-dom, see [23] for example.

Finally, Eq. (9) yields the following set of matrix
equations, where fN1_{g}t
¼ fN11; N22; N12g, and fM1g
t
¼
fM11; M22; M12g:
½S
fuper_{g}
fEg
fKg
8
<
:
9
=
;¼ jY j
f0g
fN1_{g}
fM1_{g}
8
<
:
9
=
; ð10Þ

where ½S is the stiﬀness matrix of the structure calcu-lated from Eq. (9) and from the local constitutive equation.

As a consequence, it appears that the dual variables
to macroscopic deformation fEg and fKg are
respec-tivelyjY jfN1_{g and jY jfM}1_{g, wherefrom a simple way to}

obtain the homogenized constitutive equation. Indeed, noting this equation in the form given in Eq. (7) and by successively imposing a component of ffEgt;fKgtg in

Eq. (10) to be equal to unity and the others to be zero,
displacements vEab _{and v}Kab _{are the solution u}per_{. The}

calculation of the reaction forces associated with the boundary conditions imposed on the macroscopic de-grees of freedom makes it possible to build the stiﬀness matrix in Eq. (7) column by column.

All these diﬀerent steps were implemented in a ﬁnite
element program. In practice, quadratic 3D solid ﬁnite
elements are taken to mesh the cell in order to model the
bending phenomena properly. In addition, the
unique-ness of the solution to Problem (4) is ensured by zeroing
uper _{at one node of the cell.}

Because of the one-directional periodicity of the stiﬀeners, the homogenization problems are bidimen-sional, in plane (x1; x3). However, the ﬁnite element

program was designed for more general applications (periodic panels in two directions, see Fig. 2) and the modiﬁcations mentioned above on the element matrices have only been made on the 3D solid elements. The model used was therefore fully 3D, with only one ele-ment in the direction x2. In the following, the ﬁnite

el-ement computation of the plate eﬀective properties will be called the numerical homogenization method.

We will also use an analytical homogenization method. Since the cell problems are bidimensional, ki-nematical assumptions over the thickness make it pos-sible to reduce the homogenization problem to that of a one-dimensional beam. Then, analytical expressions for the homogenized characteristics of the plate can be ob-tained [8]. Let us remark that the range of applications for such a method is narrow, because analytical ex-pressions cannot be obtained for any shape of stiﬀeners. In particular, this method will only be used here for straight stiﬀeners, the other structures being studied by numerical method. The analytical expressions of the homogenized characteristics are given in Appendix A.

We are now going to apply the numerical and ana-lytical homogenization methods described above to the diﬀerent panels shown in Fig. 1.

3. Membrane and bending behaviors of the diﬀerent structures

It is recalled that the objective of the present study is to calculate the static mechanical behavior of each structure in order to compare the stiﬀnesses of the al-veolar geometries with that of the stiﬀened panel, for a given mass.

The usual panel taken as a reference for this study is a portion of stiﬀened panel between the main girders of the steel hull of a passengers ship. This stiﬀened plate is made out of 5-mm thick steel longitudinally reinforced by bulb ﬂats HP 100 6 (see Fig. 3).

The mechanical properties for steel are E¼ 210 GPa, m¼ 0:3.

3.1. Comparison indicators

In order to avoid the tedious comparison of all the components of the overall behavior matrices obtained for the diﬀerent panels, it is useful to consider some characteristic values taken as indicators.

First, let us mention that the panel equivalent char-acteristics are determined with respect to the reference plane deﬁned by y3¼ yy3 for all the panels except the

stiﬀened one, for which the reference plane is the mid-plane of the carrier plate. On the other hand, following [7,8] and due to the symmetry properties of the cells, it can be shown that, for all the panels, the terms abcd representing respectively the membrane, membrane bending coupling and bending eﬀective stiﬀnesses in matrices ½A, ½B, ½D are zero if index 1 or 2 appears an odd number of times, and matrix ½B is zero except for the stiﬀened plate.

Considering the compliance matrices½A1and½D1, one can classically [24] deﬁne moduli Em;f

a and G m;f 12

re-spectively associated with in-plane and bending behav-iors (membrane and bending moduli):

½A1¼ 1
tref
1=Em
1 mm21=E2m 0
mm
12=Em1 1=E2m 0
0 0 1=Gm
12
2
6
4
3
7
5
½D1¼12
t3
ref
1=Ef1 m
f
21=E
f
2 0
mf12=E
f
1 1=E
f
2 0
0 0 1=Gf_{12}
2
6
4
3
7
5
ð11Þ

Direction 1 is taken perpendicular to the corrugation (see Fig. 1), and thickness tref equal to 5 mm, like the

thickness of the sheet used for the reference panel. The diﬀerent panels can then be sorted by membrane moduli (Em

1; Em2; Gm12) and by bending moduli (E f 1; E

f 2;

Gf_{12}). These quantities are directly comparable to steel
YoungÕs and shear moduli, and can readily be
inter-preted by engineers.

3.2. Implementation of the homogenization method 3.2.1. Introduction

The geometry of the reference panel is known (see Fig. 3), but that of the alveolar panels is to be deter-mined. Since our objective is to compare the ratios be-tween the equivalent stiﬀnesses and the mass of the diﬀerent structures, our methodology will be as follows.

725 5 HP 100 x 6 1 2 3 r = 4.5 r = 4.5 100 6 21.5 30˚ 3 1

After calculating the stiﬀness moduli Em;f a and G

m;f 12 of

the reference stiﬀened panel using the numerical ho-mogenization method, the panel with straight stiﬀeners will be considered. Indeed, the analytical homogeniza-tion method can be implemented on this panel, making it possible to carry out a parametric study of its diﬀerent geometric characteristics. Geometry for the panel with straight stiﬀeners will be determined such that its stiﬀ-ness moduli lie within 5% of those of the reference panel. The other panel geometries will then be set in such a way that the mass per unit area of the panels be close to that of the panel with straight stiﬀeners. Finally, the nu-merical homogenization method will be applied to all the alveolar panels.

3.2.2. Study of the panel with straight stiﬀeners

The purpose here is to determine the geometry of the panel with straight stiﬀeners according to the procedure explained above. To this aim, a parametric pre-study is made using an analytical method of homogenization (the expressions used are given in Appendix A). The parameters of this study are total thickness t of the pa-nel, thickness tf of the facings, thickness tc of the core

and distance p between two stiﬀeners (see Fig. 4). By varying these geometric parameters in turn, the others being ﬁxed, their respective inﬂuence on the panel overall membrane and bending behaviors can be as-sessed. The values that parameters t, tf, tc and p should

be given can then readily be determined, for stiﬀness moduli Em;f

a and G m;f

12 to be at least within 5% of those of

the stiﬀened panel.

After computation, it appears that bending modulus
Ef_{2} is mainly driven by panel total thickness t, and that
the three other parameters, tf; tc and p essentially aﬀect

the membrane moduli. A 60 mm thickness t is necessary
to meet the bending stiﬀness E_{2}f of the stiﬀened plate. As
for the other parameters, tf; tc and p, they must

respec-tively be set to 2.4 mm, 1 mm and 45 mm to obtain the membrane moduli Em

1 and E2mof the stiﬀened panel. One

ﬁnally gets a cell period whose geometric characteristics are deﬁned in Fig. 4.

3.2.3. Geometric deﬁnition of the three other types of alveolar panels (hat type, triangular, curvilinear)

Geometry of the other alveolar panels was set in or-der for the panelsÕ mass per unit area to be close to that

of the panel with straight stiﬀeners. Moreover, panel thickness t and facings thickness tf were taken identical

for all the structures, so as to highlight the role of the core only. The cell periods deﬁned are shown in Fig. 4. 3.2.4. Numerical homogenization of the alveolar panels

The geometric characteristics of the cell periods studied are presented Fig. 4.

These cell periods are studied using the numerical homogenization method. An example of the deformed

r S H 1 H2 T1 T2 C t = 60 mm tf= 2.4 mm p = 45 mm tc= 1 mm p = 60˚ d = 10.6 mm tc= 0.7 mm = 70˚ d = 31.4 mm tc= 0.7 mm = 60˚ tc= 0.6 mm = 40˚ tc= 1 mm tc= 0.8 mm r = 27.2 mm t d 1 3 tf tc θ θ θ θ θ θ

Fig. 4. Alveolar geometries studied.

Fig. 5. Deformed shapes obtained from solving the basic cell problems
for the panel with straight stiﬀeners: initial conﬁguration shown in
broken line, deformed shape in solid line. (a) vE11_{, (b) v}E22_{, (c) v}E12_{, (d)}

shapes corresponding to the solution of the basic cell problems is shown in Fig. 5.

The results concerning the panelsÕ stiﬀness moduli and PoissonÕs ratios in membrane and bending behav-iors are gathered in Table 1.

3.3. Results analysis

First of all, it is to be noticed that the discrepancies in the mass per unit area reach 1.2% at most. Then, com-paring the diﬀerent structures from the point of view of their ratios of eﬀective stiﬀness over mass comes down to comparing their equivalent stiﬀnesses.

As opposed to the reference stiﬀened panel, the al-veolar panels do not exhibit signiﬁcant diﬀerences in their membrane stiﬀnesses Em

1, Em2, Gm12nor in their

lon-gitudinal bending stiﬀnesses Ef_{2}. However, their bending
moduli E_{1}f are much higher (in the orthogonal plane to
corrugation) and so are the torsion moduli Gf_{12}. In fact,
the pure bending behavior of alveolar panels is
quasi-isotropic, which means that Ef_{1} and E_{2}f are on the same
order of magnitude and that Gf_{12} is within a ðEf_{=2ð1 þ}

mÞÞ ratio, where m ¼ 0:3. On the contrary, the traditional
stiﬀened plate features very diﬀerent Ef_{1} and Ef_{2} moduli:
the eﬀect of the stiﬀeners is most signiﬁcant in the
cor-rugation direction (direction 2, see Fig. 1). The stiﬀened
panel therefore exhibits a strongly anisotropic bending
behavior.

On the other hand, the comparison of the six alveolar geometries between them shows that they have almost identical eﬀective stiﬀnesses. This result reveals the prominent role played by the facings on the overall membrane and bending behaviors of an alveolar panel: as mentioned above about the straight stiﬀeners, the facings thickness drives the panel membrane behavior and the facings spacing drives the bending behavior. In comparison, the core shape has practically no inﬂuence on the membrane or bending stiﬀnesses.

Another way to pinpoint the important role played by the facings on the panel overall behavior consists in using the classical laminated plate theory to assess the equivalent behavior of a multilayered composite plate

made of two facings and one intermediate layer whose YoungÕs modulus is negligible compared to that of the facings. One obtains:

Em_{1} ¼ Em
2 ¼
2tf
href
E¼ 201:6 GPa
Gm_{12}¼ 2tf
href
G¼ 77:54 GPa
Ef_{1} ¼ Ef2 ¼
h3
ref ðhref 2tfÞ3
h3
ref
E¼ 80:31 10E3 GPa
Gf_{12}¼h
3
ref ðhref 2tfÞ3
h3
ref
G¼ 30:89 10E3 GPa
ð12Þ
Then, it appears that the core has only a signiﬁcant
contribution in the case of loads in the corrugation
di-rection and for in-plane shear of the panel.

4. Validation of the homogenization method for membrane and pure bending loadings

4.1. Presentation of the method

In order to validate the homogenization method presented in Section 3, loading cases corresponding to simple macroscopic resultant stresses will be considered. At ﬁrst, the response of the real heterogeneous panel predicted by the ﬁnite element method will be compared to the analytical solution of the same problem posed on the equivalent homogeneous plate. This procedure will make it possible to identify the equivalent characteristics of the homogeneous panel. These values will then be taken as references and will be checked against those obtained from the numerical homogenization method.

With the above objective in mind, let us consider a panel of ﬁnite dimension in one direction and of inﬁnite dimension in the perpendicular direction, so that the problem is simpliﬁed into the one-dimensional cylin-drical bending of an equivalent plate.

Table 1

Panel membrane and bending homogenized characteristics Structure (type

of stiﬀener)

Membrane behavior Bending behavior Mass per unit
area (kg/m2_{)}

Moduli (GPa) PoissonÕs ratio, mm

12 Moduli (10E3 GPa) PoissonÕs ratio, m f 12 Em 1 E m 2 G m 12 E f 1 E f 2 G f 12 Ref 213.5 254.9 80.91 0.0046 13.43 90.48 4.808 0.0008 47.64 S 205.5 253.1 77.68 0.2436 80.90 86.59 30.94 0.2803 47.31 H1 208.1 252.8 84.54 0.2469 81.91 88.20 31.68 0.2786 47.25 H2 213.1 252.7 85.54 0.2530 83.83 90.69 32.92 0.2773 47.23 T1 205.7 256.1 89.94 0.2409 80.90 86.88 30.93 0.2794 47.87 T2 205.3 251.7 82.47 0.2447 80.84 86.35 30.91 0.2808 47.05 C 205.4 254.4 85.76 0.2423 81.07 89.68 30.89 0.2712 47.54 Moduli Em;f a and G m;f

As far as the ﬁnite element model of the real panel is concerned, the cylindrical bending conditions are im-posed in the following way:

• for the study in plane 13, only one ﬁnite element is taken in direction 2 since the structure is invariant in this direction, and the translation and rotation de-grees of freedom of two nodes A and B facing each other in direction 2 are made equal. See Fig. 6(a) for the panel with 60 (T2) triangular stiﬀeners. All the following ﬁnite element analyses were run with the commercial package Samcef [25]. The meshes were made of 4-node Mindlin elements, and a perfect bonding between the facings and the core was as-sumed.

• for the study in plane 23, one considers a one-period length in direction 1 because the structure is not in-variant in this direction. The cylindrical bending con-ditions are written at nodes A and B located on the edges of the cell period. See Fig. 6(b).

4.2. Membrane loading

The loading and boundary conditions on the heter-ogeneous panel in plane 13 are described in Fig. 7(a).

The analysis is made on a 10-period model, and force F is calculated such that N11¼ 10E3 N/mm.

The response of the structure is then estimated using the ﬁnite element method, and half-sum uFEof the axial

displacements of the two facings at a given position x1is

computed for comparison with the analytical solution of the homogeneous equivalent plate problem.

The membrane and bending behaviors of the equiv-alent homogeneous plate being uncoupled, and matrix ½A in Eq. (7) being such that A1112¼ A2212¼ 0, the

an-alytical solution is given as: u¼ N11

A1111

x1 ð13Þ

As an example, the results obtained for the panel with T2 triangular stiﬀeners are presented. If uFEis plotted as

a function of x1, one gets the curve shown in Fig. 8(a),

and this curve can very well be approximated as a straight line. In addition, the slope of this straight line can be identiﬁed using the least-square method, which yields A1111¼ 1:108 10E6 N/mm.

On the other hand, according to the results about the
T2 panel (see Table 1), the value obtained from
ho-mogenization is:
A1111¼ href
Em
1
1 ðmm
12Þ
2 Em_{2}
Em
1
¼ 1:108 10E6 N=mm ð14Þ

There is obviously an excellent agreement between the value of the eﬀective stiﬀness determined by the ﬁnite element analysis of the real heterogeneous panel and that calculated by the homogenization method.

4.3. Pure bending loading

In plane 13, the boundary conditions and forces shown in Fig. 7(b) impose a pure bending loading. Force F is such that M11¼ 1000 N.

The results given by the ﬁnite element method are analyzed after determining wFE deﬁned as the half-sum

of the deﬂections of the two facings at a given position x1.

For the homogeneous plate, matrix ½D in Eq. (7) being such that D1112¼ D2212¼ 0, the analytical solution

Fig. 6. Finite element model used for the study (a) in plane 13 and (b) in plane 23.

Fig. 7. Loading and boundary conditions in (a) membrane, (b) pure bending and (c) simple bending.

Fig. 8. Panel response with T2 stiﬀeners in (a) membrane, (b) pure bending loadings.

is given as (where ‘ represents the length of the panel studied):

w¼ M11 2D1111

x1ð‘ x1Þ ð15Þ

For a 10-period-long panel with T2 stiﬀeners, the results for wFE are shown in Fig. 8(b). By determining

coeﬃcient D1111such that Eq. (15) best represents wFEin

the least-square sense, one gets D1111¼ 9:195 10E8

Nmm. And the value obtained from homogenization is
(see Table 1):
D1111¼
ðhrefÞ
3
12
Ef_{1}
1 ðmf12Þ
2 E_{2}f
E_{1}f
¼ 9:195 10E8 N mm
ð16Þ
Like for membrane loading, there is an excellent
agreement between the bending eﬀective stiﬀness
calcu-lated on the real panel and that obtained from the
ho-mogenization method.

These results are as satisfactory as those shown above for the other membrane and bending characteristics, and this holds for all the panel types studied here. Another example of the accuracy of the homogenization method used in the present paper can be found in [9,10] where the example of a honeycomb plate made of steel is treated. In order to show the applicability of the ho-mogenization method to composite structures, an ex-ample with FRP materials is treated in Section 5.

5. Homogenization of a ﬁber-reinforced plastic honey-comb sandwich panel

As an example of FRP structure, we consider the case of a honeycomb sandwich panel for highway decks,

which was studied in [18]. This structural panel consists of a sinusoidal wave core conﬁguration in the plane, extending vertically between face laminates. Thus, the panel exhibits in-plane periodic structure, and Fig. 9(a) presents its basic cell, the upper facing being not rep-resented.

The geometric data of the basic cell are:

• thicknesses, total: t ¼ 126:52 mm, face laminates: tf ¼

10:87 mm, core: tc¼ 2:28 mm,

• in plane dimensions: p1¼ 101:6 mm, p2¼ 110:72

mm.

The core has a sinusoidal wave conﬁguration, with an amplitude 2h (with h¼ 25:4 mm) and p2¼ 4h þ 4tc, see

Fig. 9(a), one half of the core wall being modeled on the basic cell boundaries normal to direction 2.

The core and face laminates are constituted with E-glass ﬁbers and polyester resin. The core is made with a single layer of continuous strand mat with continuous randomly oriented ﬁbers, while the face laminates in-clude four types of ﬁber layers, see [18]. However, to solve the basic cell problems, it is indeed suﬃcient to consider the core (with its real sinusoidal geometry) and laminates as homogeneous layers. So we use here the equivalent properties given in [18], and obtained from a micromechanics approach for each layer, com-bined with classical lamination theory for the facings. These material properties are listed in Tables 2 and 3, and are taken from Tables 3 and 4 of [18] (in Table 2, the direction 3 is normal to the core layer, while in Table 3, the directions 1 and 2 correspond to those of Fig. 9(a)).

Let us mention that given that the basic cell problems are 3D, a 3D constitutive behavior has to be deﬁned from the data of Tables 2 and 3. So the following assump-tions were made for the core properties (E3¼ E1¼ E2,

G13¼ G23 and m13¼ m23), while for the face laminates we

took E3¼ E2, m13¼ m23¼ m12 and G12¼ G23¼ G13. One

can easily verify that these assumptions have a negligible eﬀect on eﬀective properties since itÕs mainly the in-plane behavior of the core and the facings which is involved in the loadings of the basic cell problems. The mesh used for the numerical homogenization method is shown in Fig. 9(b).

From (11), with tref ¼ 126:52 mm i.e. the panel total

thickness, the eﬀective moduli of the sandwich structure are computed. Table 4 shows the results obtained with the numerical 3D homogenization method, in com-parison to those of [18]. In [18], in a ﬁrst step, an an-alytical solution is used for the evaluation of equivalent core properties, and then classical lamination theory provides the sandwich panel eﬀective properties, con-sidering the structure as a three layers laminated sys-tem. Therefore, skin core interactions are neglected, which yields underestimate of stiﬀness, as noted in [11]. These eﬀects are rigorously taken into account in the method used in this paper, through the 3D modeling used in the basic cell problems. From Table 4, it may be seen that there is not a signiﬁcant diﬀerence between our approach and the results of [18]. However, our approach is more accurate because it enables to com-pute local distribution of stresses. Thus, once the computations are made on the equivalent homogeneous plate, these local stresses are simply obtained by a lin-ear combination of the obtained macroscopic strains and the solution of the basic cell problems (see e.g. Fig. 10 the von-Mises stress distribution for a given unit curvature).

6. Behavior of the structures in transverse shear

6.1. Introduction

Owing to what has been shown above, it can be stated that the homogenization method proves to be very ac-curate to provide the characteristics of an equivalent Kirchhoﬀ Love plate. Nevertheless, it is not guaranteed that a Kirchhoﬀ Love model is suﬃcient to describe the overall behavior of a sandwich panel. In order to in-vestigate this question, let us consider a simple bending loading, still under the assumption of cylindrical bend-ing.

The analysis is performed on a 10-period-long panel, in plane 13, when condition ~uu¼ ~00 is imposed at all the nodes in the cross-section of the origin, see Fig. 7(c). Force F is taken such that Q1¼ 10E3 N/mm.

When the analysis of the heterogeneous panel is done, facings average deﬂection wFE is determined and

com-pared with that given by the analytical solution to the Kirchhoﬀ Love plate problem, i.e.:

wKL ¼ Q1 D1111 x3 1 6 ‘x 2 1 2 ð17Þ The plot shown in Fig. 11(a) represents the results obtained for a panel with T2 stiﬀeners. One can notice a discrepancy between the two solutions. This discrepancy

Table 4

Eﬀective moduli for the FRP honeycomb sandwich panel

Membrane behavior Bending behavior Moduli (GPa) PoissonÕs ratio, mm

12 Moduli (GPa) PoissonÕs ratio, m f 12 Em 1 E m 2 G m 12 E f 1 E f 2 G f 12 Numerical homog. 3.834 2.280 0.687 0.312 8.807 5.613 1.680 0.307 Ref. [18] 3.813 2.206 0.648 0.303 8.777 5.537 1.627 0.301

Fig. 10. Von Mises stress (MPa) contour lines on the deformed shape
vK11_{.}

Table 2

Engineering constants for the core material

E1(GPa) E2(GPa) G12(GPa) G23(GPa) m12 m23

11.79 11.79 4.21 2.97 0.402 0.388

Table 3

Engineering constants for face laminates

E1(GPa) E2(GPa) G12(GPa) m12

is not signiﬁcant for this type of stiﬀeners but is im-portant for stiﬀeners that are straight (see Fig. 11(b)), curvilinear, or in hat shape, although all the structures studied have almost the same equivalent membrane and bending characteristics.

It appears that a Kirchhoﬀ Love model is not com-pletely satisfactory, and it is therefore necessary to take into account the transverse shear eﬀects. As has been seen in the last results, these characteristics seem to be very sensitive to the core shape.

The problem is then to deﬁne an homogenization method for the transverse shear behavior.

Starting from 3D elastic problem, the asymptotic expansion method enables to recover, at the leading order, the Kirchhoﬀ Love model. It can indeed be shown that the transverse shear forces associated with stresses r1

13and r 1

23are zero. As a result, solving the cell

problems described in Eq. (4) does not provide any in-formation on the plates stiﬀness in transverse shear.

Reﬁned plate theories, taking into account transverse shear eﬀects, can be obtained using the asymptotic ex-pansion method, including the higher-order terms of the expansion [26]. Such theories are complex, since they involved higher derivatives, and are therefore not used by engineers. This justiﬁes attempts to derive an as-ymptotically correct Reissner Mindlin second order theory [27]. However, such a process isnÕt straightfor-ward, because one has to choose the asymptotical cor-rectness criterion. Moreover a higher-order microscopic problem needs to be solved. Consequently, this method will not be used in this paper.

Another way to proceed to obtain an equivalent Reissner Mindlin plate is to use the homogenization method proposed in [28]. Its starting point is the bidi-mensional equations of a Reissner Mindlin plate with periodic coeﬃcients. As a consequence, the downside of this method is that the 3D behavior of the plate is only roughly taken into account, since it is a priori assumed that the heterogeneous 3D panel behaves like a hetero-geneous Reissner Mindlin plate. The application ﬁeld of this method is therefore limited to cells whose in-plane dimensions are very small compared to their thickness [8,15,16], i.e. for e e, whereas for the example under consideration here, e e. It will be seen below that this

method is inappropriate as far as the determination of the transverse shear stiﬀness is concerned.

It is then necessary to resort to another type of ap-proach.

In the present work, we will use a numerical method to determine the corrugated core sandwich panel equivalent stiﬀness in transverse shear. Assuming the overall behavior being of Reissner Mindlin type, the transverse shear stiﬀness will be identiﬁed from the re-sults obtained about a panel made of several cell peri-ods. This is a diﬀerence from the method used for the homogenization of membrane and bending behaviors, where the ﬁnite element model only represented one period.

Let us mention that in the following, our study will be restricted to the corrugated sandwich panels of Fig. 1. However, the method proposed in this paper is also valid for the FRP honeycomb sandwich panel of Section 5 (in [18], its shown that a Timoshenko beam model is in good agreement with experimental data for three-point and four-point bendings).

6.2. Principle of the method

Let us re-consider the calculation made at the ginning of this section, assuming that the overall be-havior in transverse shear and the membrane and bending behaviors are uncoupled, and that the associ-ated stiﬀness matrix is diagonal, such that:

Q1 Q2 ¼ k1 0 0 k2 w;1þ h2 w;2 h1 ð18Þ where h1 and h2 denote rotations about the x1 and x2

axes, respectively.

Then, the analytical solution to the equivalent ho-mogeneous Reissner Mindlin plate problem is given by: wRM¼ Q1 D1111 x3 1 6 ‘x 2 1 2 þQ1x1 k1 ¼ wKLþ Q1x1 k1 ð19Þ One can further deﬁne from the ﬁnite element anal-ysis of the heterogeneous panel:

w _{FE}ðx1Þ ¼ wFEþ
Q1
D1111
x3
1
6
‘x
2
1
2
¼ wFE wKL ð20Þ

calculated with the value of D1111 obtained from the

homogenization method, and the accuracy of which has been established in Section 4.3. It is therefore assumed that Eq. (7) describes the membrane and bending be-haviors of the equivalent Reissner Mindlin plate, when curvatures fK11; K22;2K12g are substituted with fh2;1;

h1;2;h2;2 h1;1g.

Then, if w

FEis plotted as a function of x1, the graphs

shown in Fig. 12(a) and (b) are obtained for T2 and straight stiﬀeners respectively:

A straight line is found in both cases, and this shows, from Eqs. (19) and (20), that the panel overall response Fig. 11. Panel response in simple bending loadings (a) T2 stiﬀeners, (b)

is similar to that predicted by a Reissner Mindlin model. It also provides a simple way to identify k1from

the slope of the straight line using the least-square method.

However, one can notice that for T2 stiﬀeners, the diﬀerence between w

FEand wFEis only about 10%. Since

w

FE is obtained from the homogenized bending

char-acteristics of the panel, one may want to diminish the relative importance of wKL in Eq. (20). Then, the length

of the structure will be decreased so that w

FE is at least

20% lower than wFEat the loaded tip of the panel.

For the study in plane 13, this has led us to generally consider 5-period-long panels, except for the T1 panel, where 3 periods are taken.

In plane 23, the same procedure applies, and
ac-cording to the same criterion, 5-period-long panels are
considered, except for T1 and H2 panels, where 4
peri-ods are studied. The boundary condition ~uu¼ ~00 is
im-posed at all the nodes in the cross-section of the origin
(core and facings). One ﬁnally uses the expression:
w _{FE}ðx2Þ ¼ wFEþ
Q2
D2222
x3
2
6
‘x
2
2
2
¼ wFEþ wKL ð21Þ

knowing that the analytical solution w _{is given by:}

w ¼Q2x2 k2

ð22Þ

6.3. Results

For all the panels studied here, straight lines very well approximate the curves w

FEðx1Þ in plane 13 and w FEðx2Þ

in plane 23 obtained from the method described above. In turn, the values of k1and k2can be calculated. From

these values, and using reference thickness href ¼ 5 mm,

we may deﬁne engineering constants in the form of shear moduli G13and G23 such that:

k1¼

5

6hrefG13; k2¼ 5

6hrefG23 ð23Þ The values calculated from Eq. (23) are gathered in Table 5.

Let us note that if the homogenization method [28] mentioned at the beginning of Section 6 is used (see the corresponding analytical expressions given in Appendix

A) one gets G13¼ 0:792 GPa and G23¼ 0:974 GPa for

straight stiﬀener. These values are very far from the reference values obtained from the ﬁnite element ana-lyses. Thus, such a homogenization method should not be applied to the type of panels considered here.

The values in Table 5 are to be compared with the shear modulus of steel G¼ 0:808 GPa, this value being a ﬁrst approximation of the stiﬀened panel equivalent moduli in planes 13 and 23. Indeed, it can be stated that the stiﬀness in transverse shear of the stiﬀened panel is at least that of the underlying steel plate.

6.4. Results analysis

Compared to the case of the membrane and bending equivalent characteristics, signiﬁcant diﬀerences can be noted.

First of all, the value of G13is very diﬀerent from one

panel to the other, and can be up to 1000 times lower than that of the reference stiﬀened panel. The results in plane 23 are less scattered, and the stiﬀness of the sandwich panels is on the same order of magnitude as that of the stiﬀened panel, although lower.

As a result, the alveolar panels have a strong aniso-tropic behavior in transverse shear, except for panels with triangular-shaped stiﬀeners. It appears then that the core shape has a strong inﬂuence on the value of modulus G13, and that T2 triangular stiﬀeners at 60 give

the best transverse shear stiﬀness for sandwich panels. Finally, the values obtained show that it is necessary to use a Reissner Mindlin plate model, even for the stiﬀest panel (see Fig. 11(a)).

7. Conclusions

In this work, we have applied a periodic homogeni-zation method to determine the equivalent membrane and pure bending characteristics of periodic plates. This method requires a few developments in a ﬁnite element package, and is then very easy to implement. As dem-onstrated in Section 4, this method yields very good results. Moreover, this method can be applied to many Table 5

Panels homogenized characteristics in transverse shear Structure (type of

stiﬀener)

Equivalent shear moduli (GPa)

G13 G23 S 0.207 240 H1 22.3 149 H2 1.58 139 T1 164 91.4 T2 123 164 C 0.400 95.3

Moduli G13and G23for a 5 mm thick equivalent homogeneous plate.

Fig. 12. Analysis of results in simple bending (a) T2 stiﬀeners, (b) straight stiﬀeners.

engineering structures, such as composite structures, see Section 5.

However, the method does not make possible the evaluation of the transverse shear stiﬀness of sandwich panels. Therefore, we used another approach based on calculations in cylindrical bending. Then, after verifying that the panel overall response was in agreement with a Reissner Mindlin model, its transverse shear stiﬀness was identiﬁed from the results of the calculations.

This study allows to compare diﬀerent types of alve-olar structures with traditional stiﬀened structures, with a view to their applications in shipbuilding. Several conclusions can be drawn from the present work.

For a given mass per unit area, alveolar panels pre-sent a better overall bending stiﬀness than traditional stiﬀened panels. On the opposite, eﬀective membrane stiﬀnesses are similar for all the panels. As a result, a weight reduction is possible, especially as far as the bending characteristics are concerned.

For the overall membrane and pure bending behav-iors, the two driving parameters are the thickness of the facings and their spacing, whereas stiﬀeners geometry has only a minor inﬂuence. However, the equivalent behavior in transverse shear is very dependent on the stiﬀeners geometry, and it appears that triangular stiﬀ-eners have the best characteristics.

Finally, the important role played by shear stress in the behavior of such sandwich structures was high-lighted.

Thanks to the methods presented in this work, we can determine the panelsÕ eﬀective characteristics according to a Reissner Mindlin plate. This will make it possible to model the alveolar panels as equivalent homogeneous plates, and will reduce the computation time when the ﬁnite element analysis is made on the whole ship.

Acknowledgement

The authors wish to thank Dr S. Bourgeois (L.M.A., Marseille, France) for the fruitful discussions they had with him on this subject.

Appendix A

According to [8], here are reported the analytical expressions for the homogenized characteristics of a panel with straight stiﬀeners (see Fig. 4(a)). It is recalled that the membrane bending coupling matrix½B is zero, that matrices½A and ½D are symmetric, and that their terms with indices abcd are zero if index 1 or 2 appears an odd number of times.

By noting, c1¼ tc=p and c2¼ 1 c1, one gets, for

membrane stiﬀnesses: A1111¼ c1 t þ c2 2tf 1 E 1 m2 A1122¼ mA1111 A2222¼ ðc1tþ 2c2tfÞE þ m2A1111 A1212¼ c1 t þc2 2tf 1 E 2ð1 þ mÞ ðA:1Þ

and for bending stiﬀnesses
D1111¼
2
3
8c1
t3 þ
8c2
t3_{ ðt 2t}
fÞ
3
!
E
1 m2
D1122¼ mD1111
D2222¼
2
3
h3
8 c2
h
2
ep
3!
Eþ m2_{D}
1111
D1212¼
2
3
c1t3
8 þ c2ð1 3f þ 3f
2_{Þt}3
f
t
2 tf
6
T
!
ðA:2Þ
with
T ¼ p lh
3
8 coth
2ltc
t
þ l0_{e}2
pcoth
l00_{ðp t}
cÞ
tf
;
f¼ t
2tf
; l¼ 3k
p
2 ; l
0_{¼ ð1 3f þ 3f}2
Þ1=2l;
l00¼ ð1 3f þ 3f2_{Þ}1=2
l ðA:3Þ

and where k is the shape factor used for shear stiﬀness, taken here to be equal to 5/6.

As for the equivalent stiﬀness in transverse shear obtained by homogenization of a Reissner Mindlin plate problem, the following holds, according to [8]:

k1¼
5
6
c1
t
þc2
2tf
1 _{E}
2ð1 þ mÞ;
k2¼
5
6ðc1tþ 2c2tfÞ
E
2ð1 þ mÞ ðA:4Þ
References

[1] Noor AK, Burton WS, Bert CW. Computational models for sandwich panels and shells. Appl Mech Rev1995;155(3):155 99. [2] Triplett MH, Schonberg WP. Static and dynamic ﬁnite element analysis of honeycomb core sandwich structures. Struct Eng Mech 1998;6(1):95 113.

[3] Burton WS, Noor AK. Assessment of continuum models for sandwich panel honeycomb cores. Comput Meth Appl Mech Eng 1997;145(3 4):341 60.

[4] Hohe J, Becker W. Eﬀective stress strain relations for two dimensional cellular sandwich cores: Homogenization, material models, and properties. Appl Mech Rev2002;55(1):61 87. [5] Ko WL. Elastic constants for superplastically formed/diﬀusion

bonded sandwich structures. AIAA J 1980;18(8):986 7. [6] Nordstrand T, Carlsson LA, Allen HG. Transverse shear stiﬀness

[7] Caillerie D. Thin elastic and periodic plates. Math Meth Appl Sci 1984;6:159 91.

[8] Lewinski T, Telega JJ. Plates, laminates and shells. Asymptotic analysis and homogenization. Singapore: World Scientiﬁc; 1999. [9] Bourgeois S, Cartraud P, Deebordes O. Homogenization of

periodic sandwiches. In: Vautrin A, editor. Mechanics of sand wich structures. Dordrecht: Kluwer; 1998. p. 131 8.

[10] Bourgeois S. Modeelisation numeerique des panneaux structuraux leegers. Ph.D. Thesis. University Aix Marseille II, 1997.

[11] Xu XF, Qiao P. Homogenized elastic properties of honeycomb sandwich with skin eﬀect. Int J Solids Struct 2002;39:2153 88. [12] Kohn RV, Vogelius M. A new model for thin plates with rapidly

varying thickness. Int J Solids Struct 1984;20:333 50.

[13] Hohe J, Becker W. A reﬁned analysis of the eﬀective elasticity tensor for general cellular sandwich cores. Int J Solids Struct 2001;38:3689 717.

[14] Parton VZ, Kudryavtsev BA. Engineering mechanics of compos ite structures. Boca Raton, FL: CRC Press; 1993.

[15] KalamkarovAL. Composite and reinforced elements of construc tion. New York: Wiley; 1992.

[16] KalamkarovAL, KolpakovAG. Analysis, design and optimiza tion of composite structures. Chichester: Wiley; 1997.

[17] Mouftakir L. Homogeeneeisation des structures onduleees. Ph.D. Thesis. University Metz, 1996.

[18] Davalos JF, Qiao P, Xu XF, Robinson J, Barth KE. Modeling and characterization of ﬁber reinforced plastic honeycomb sand wich panels for highway bridge applications. Compos Struct 2001;52:441 52.

[19] Leenee F. Contribution a lÕeetude des mateeriaux composites et de leur endommagement. Thesis. University Paris 6, 1984.

[20] Deebordes O, Licht C, Marigo JJ, Mialon P, Michel JC, Suquet P. Calcul des charges limites de structures fortement heeteerogeenes. In: Grellier JP, editor. Tendances actuelles en calcul des structures. Paris: Pluralis; 1985. p. 56 70.

[21] Devries F, Dumontet H, Duvaut G, Leenee F. Homogenization and damage for composite structures. Int J Numer Meth Eng 1989; 27:285 98.

[22] Guedes JM, Kikuchi N. Preprocessing and postprocessing for materials based on the homogenization method with adaptative ﬁnite element methods. Comput Meth Appl Mech Eng 1990;83: 143 98.

[23] Michel JC, Moulinec H, Suquet P. Eﬀective properties of composite materials with periodic microstructure: a computa tional approach. Comput Meth Appl Mech Eng 1999;172(1 4):109 43.

[24] Tsai SW. Theory of composites design. Dayton: Think Compos ites; 1992.

[25] Samtech. Samcef elements user manual, version 7.1, 1997. [26] Goldenveizer AL, Kaplunov JD, Nolde EV. On Timoshenko

Reissner type theories of plates and shells. Int J Solids Struct 1993;30(5):675 94.

[27] Sutyrin VG. Derivation of plate theory accounting asymptotically correct shear deformation. J Appl Mech 1997;64:905 15. [28] Tadlaoui A, Tapiero R. Calcul par homogeeneeisation des micro

contraintes dans une plaque heeteerogeene dans son eepaisseur. J Meec Theeor Appl 1988;7:573 95.